Hindawi Publishing Corporation BioMed Research International Volume 2016, Article ID 7576942, 7 pages http://dx.doi.org/10.1155/2016/7576942
Research Article Effect of Surface Treatment on Shear Bond Strength between Resin Cement and Ce-TZP/Al2O3 Jong-Eun Kim,1 Jee-Hwan Kim,1 June-Sung Shim,1 Byoung-Duck Roh,2 and Yooseok Shin2 1
Department of Prosthodontics, College of Dentistry, Yonsei University, Seoul 03722, Republic of Korea Department of Conservative Dentistry, Oral Science Research Center, College of Dentistry, Yonsei University, Seoul 03722, Republic of Korea
Correspondence should be addressed to Yooseok Shin; [email protected]
Received 1 February 2016; Revised 28 April 2016; Accepted 22 May 2016 Academic Editor: Salvatore Sauro Copyright © 2016 Jong-Eun Kim et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited. Purpose. Although several studies evaluating the mechanical properties of Ce-TZP/Al2 O3 have been published, to date, no study has been published investigating the bonding protocol between Ce-TZP/Al2 O3 and resin cement. The aim of this study was to evaluate the shear bond strength to air-abraded Ce-TZP/Al2 O3 when primers and two different cement types were used. Materials and Methods. Two types of zirconia (Y-TZP and Ce-TZP/Al2 O3 ) specimens were further divided into four subgroups according to primer application and the cement used. Shear bond strength was measured after water storage for 3 days or 5,000 times thermocycling for artificial aging. Results. The Y-TZP block showed significantly higher shear bond strength than the Ce-TZP/Al2 O3 block generally. Primer application promoted high bond strength and less effect on bond strength reduction after thermocycling, regardless of the type of cement, zirconia block, or aging time. Conclusions. Depending on the type of the primer or resin cement used after air-abrasion, different wettability of the zirconia surface can be observed. Application of primer affected the values of shear bond strength after the thermocycling procedure. In the case of using the same bonding protocol, Y-TZP could obtain significantly higher bond strength compared with Ce-TZP/Al2 O3 .
1. Introduction Metal-ceramic restorations are among the most commonly used treatment options in fixed prosthodontics. However, their drawbacks include discoloration due to the metal frame showing at the gingival margin, opaque shade unlike natural teeth, and possible metal allergy . The interest in zirconia as a dental restorative material is rapidly increasing. Zirconia has biocompatibility and excellent mechanical properties such as high fracture resistance. It also has shading similar to natural teeth, and it is possible to fabricate natural-looking esthetic restorations. In particular, with the recent advances in CAD/CAM systems, restorations with ceramic build-up on a zirconia framework and restorations composed totally of zirconia are commonly used in daily dental practice. For these reasons, zirconia is receiving a spotlight as a nonmetal restoration material that could replace metal-ceramic restorations [2–7].
Yttrium-stabilized tetragonal zirconia (Y-TZP) is a polycrystalline ceramic with three crystal phases: monoclinic, tetragonal, and cubic. Yttrium oxide controls the volume expansion and stabilizes the crystal such that the tetragonal phase can be maintained at room temperature [5, 8]. The characteristic that distinguishes zirconia from other ceramics is that when a crack initiates and propagates because of external forces, the tetragonal phase around the crack can transform to monoclinic phase. Such transformation causes 3–5% volume expansion, and the compressive stress layer around the crack may stop the spread of the crack [7, 9, 10]. However, one of the drawbacks is that, in the oral environment where the material is consistently exposed to moisture, low temperature degradation occurs. This effect deteriorates the mechanical properties of zirconia [11, 12]. Zirconia is chemically and biologically inert, but it is difficult to obtain predictable bonding in clinical dental use [4, 6, 7]. For glass ceramics, etching with hydrofluoric acid
BioMed Research International
Y-TZP ceramic block Ce-TZP ceramic block
No primer Airborne abrasion
Z-Prime Plus primer
RelyX U200 cement
5,000 times thermocycling
Figure 1: Flowchart of the zirconia block surface treatments.
is the standard protocol, but zirconia is resistant to acidetching as it contains less glass and is mainly composed of crystal [13–15]. Consequently, micromechanical bonding through air-abrasion, roughening by diamond rotary instruments, and chemical bonding through primer application have been recommended [7, 16, 17]. Roughening the zirconia surface through airborne abrasion with 50 𝜇m Al2 O3 particles increases the shear bond strength of resin cement [18, 19]. Strategies to roughen the surface and obtain chemical bonding have led to the development of primer and luting cement. Various resin bond strength studies with the application of methylacryloyloxydecyl dihydrogenphosphate (MDP) monomers after airborne abrasion were performed, and such protocols have been used clinically. In prosthodontics, MDP-containing resin cement is also used . Cerium oxide can also be used for tetragonal phase stabilization [10, 20]. Recently a Ce-TZP/Al2 O3 nanocomposite that contains alumina has been developed. Alumina was interpenetrated with zirconia to enhance the strength of the Ce-TZP/Al2 O3 nanocomposite, and it consists of 10 mol% Ce-TZP and 30 vol% Al2 O3 [11, 21, 22]. Equally distributed Al2 O3 improves the hardness, elastic modulus, and stability in moist environments [23, 24]. The Ce-TZP/Al2 O3 nanocomposite has higher fracture resistance compared to conventional Y-TZP. While Y-TZP consists of homogenous grain, the Ce-TZP/Al2 O3 nanocomposite has an interpenetrated intergranular nanostructure. Nanometer-sized Al2 O3 particles are located in submicron-level ZrO2 grains, and the ZrO2 particles are located in Al2 O3 grains. This structure improves the strength of Ce-TZP/Al2 O3 [25, 26]. In addition, it is more resistant to low temperature degradation (LTD) in a moist environment compared to Y-TZP and has shown satisfactory results in terms of phase transformation and mechanical properties . While there have been many studies regarding adhesion to zirconia and there have been reports on the mechanical properties of Ce-TZP/Al2 O3 , studies on adhesion of CeTZP/Al2 O3 have been scarce. The purpose of this study was to compare the shear bond strength to air-abraded Y-TZP and Ce-TZP/Al2 O3 when primers and two different cement types were used.
2. Materials and Methods 2.1. Zirconia Specimen Fabrication and Surface Treatment. Zirconia discs were sectioned to fabricate specimens after a sintering process. The specimens were embedded in polyethylene molds with cold curing resin (Vertex Dental,
Table 1: Experimental materials used in this study. Material
NanoZR (Ce-TZP/Al2 O3 )
Manufacturer Noritake Dental Supply Co., Ltd., Japan Panasonic Health Care, Japan
Bisco Inc., Schaumburg, IL
RelyX U200 cement G-Cem linkace cement
3M ESPE, USA GC Corp., Japan
Katana Zirconia (Y-TZP) Zirconia
Singapore). One side of the disc was exposed and polished with 600-grit silicon carbide paper under water irrigation. After polishing, the blocks were put in an ultrasonic waterbath filled with tap water. The surface treatment method is described in detail in Figure 1, and the materials used in the study are shown in Table 1. Airborne abrasion was performed with 50 𝜇m sized Al2 O3 particles with 3.5-bar pressure at 10 mm distance for 15 seconds. Afterwards, additional surface treatment was performed according to the experimental group, and cementation was performed with resin cement. The zirconia specimens were divided into two groups: Y-TZP (Katana Zirconia; Noritake Dental Supply Co., Ltd., Japan) and Ce-TZP/Al2 O3 (NanoZR; Panasonic Health Care, Japan). All specimen surfaces were treated with airborne abrasion, and they were further divided into four subgroups according to primer application and the cement used: (1) group NG: cemented with G-Cem (GC Corp., Japan) without any primer application; (2) group NU: cemented with RelyX U200 (3M ESPE, Seefeld, Germany) without any primer application; (3) group PG: cemented with G-Cem linkace cement after Z-Prime Plus primer (Bisco Inc., Schaumburg, IL) application; (4) group PU: cemented with RelyX U200 after Z-Prime Plus primer application. One hundred sixty specimens in total were divided into 16 groups of 10 specimens each. Primer and resin cement application were performed according to the manufacturer’s instruction, and resin cement was applied to a plastic mold (Ultradent Jig; Ultradent Products, South Jordan, USA) to place the resin cement on the zirconia surface (bonding area 4.45 mm2 ). The plastic mold containing resin composite cement was placed on the zirconia surface and light-cured with a 1200 mW LED light curing unit (DB-686 Cappu LED Curing Light; Bisco Asia, Seoul, Korea). After light curing from 4 different directions for 20 seconds each, 80 specimens were left to further polymerize at room temperature (23 ± 1∘ C) for one hour and then kept in a water bath containing
BioMed Research International
Figure 2: SEM of the surface of the specimens after air-abrasion with 3.5-bar pressure: (a) Ce-TZP/Al2 O3 block; (b) Y-TZP block. Table 2: Median shear bond strength in MPa to zirconia surfaces before and after thermocycling (𝑝 < 0.05). Thermocycling
Katana (Y-TZP) NanoZR (Ce-TZP/Al2 O3 )
Katana (Y-TZP) NanoZR (Ce-TZP/Al2 O3 )
30.24A a 𝛼 22.89A b 𝛽
19.09B a 𝛽 14.12B a
No primer RelyX U200 𝛼
14.71C a 𝛼 14.24B a 𝛼
16.46B a 𝛼 12.27B a
Z-Prime Plus G-Cem RelyX U200 𝛼
25.21AB a 𝛼 20.48AB b 𝛼
23.60AB a 𝛽 16.15B b
22.56B a 𝛼 24.59A a 𝛼
29.69A a 𝛼 26.02A a
Note: statistical differences are indicated by different superscript upper case letters (within a column for the same zirconia block and ageing process) or by different subscript lower case letters (within a row for the same surface treatment and aging process). Letters 𝛼𝛽 in superscript reflect significant differences within a row for assessing effects of thermocycling within the same zirconia block.
tap water at 37∘ C for 3 days. The other 80 specimens were thermally cycled with 5,000 cycles between 5∘ C and 55∘ C and a dwell time of 30 seconds. 2.2. Shear Bond Strength Test. Shear bond strength was measured using a shear bond tester (Bisco Inc., Schaumburg, IL, USA). The crosshead speed was set at 0.5 mm/min. The force was applied to the adhesion surface of the specimen, and the maximum fracture strength was measured in N. The measuring data were converted into MPa by dividing by the bonding area. 2.3. SEM Analysis. The surface of the specimens after airabrasion with 3.5-bar pressure was analyzed by scanning electron microscopy (SEM) (Figure 2). The zirconia blocks were mounted after carbon adhesive application and coated with gold-palladium. Representative images were obtained from each group at 2,000x magnification. 2.4. Failure Mode Analysis. The fractured specimen interface was analyzed with an optical microscope using 10.0x magnification. The failure mode was classified as one of the following: (1) adhesive failure: failure at the interface between zirconia and resin cement; (2) cohesive failure: failure within resin; (3) mixed failure: combination of adhesive and cohesive failure.
2.5. Statistical Analysis. Statistical analysis was performed with SPSS v23.0 (SPSS Inc., Chicago, IL, USA) software. Three-way ANOVA analysis was performed to see the influence of the following factors: aging time, type of zirconia block, and surface treatments and their interaction on mean SBS (𝑝 < 0.05). The data were separated with respect to aging time and type of zirconia block for statistical analysis by one-way ANOVA with regard to the surface treatments used followed by a post hoc Bonferroni test (𝑝 < 0.05).
3. Results 3.1. Shear Bond Strength of Resin Cement to Y-TZP and CeTZP/Al2 O3 Ceramic. The mean bond strength values according to different zirconia blocks, bonding materials, and aging time are shown in Table 2. Three-way ANOVA showed that the type of zirconia block, bonding material, and aging time have a significant effect on shear bond strength (𝑝 < 0.05). A significant interaction between aging time and bonding material used was observed. However, significant interactions between other factors were not observed: aging time and type of zirconia block (𝑝 > 0.05), bonding material and type of zirconia block (𝑝 > 0.05), and aging time × type of zirconia block × bonding material (𝑝 > 0.05).
BioMed Research International 100 90 80 70 (%)
60 50 40 30 20 10 0 NG NU
Adhesive fracture Mixed fracture
Figure 3: The failure modes of shear bond tests before and after thermocycling. NG (no primer and G-Cem), NU (no primer and RelyX U200), PG (Z-Prime Plus primer and G-Cem), and PU (Z-Prime Plus primer and RelyX U200).
When the same surface treatment method and cement were used, there was a significant difference between the YTZP and Ce-TZP/Al2 O3 blocks. The Y-TZP block showed significantly higher shear bond strength than the Ce-TZP/Al2 O3 block generally. In the same zirconia block and aging time, G-Cem linkace cement showed higher bond strength than RelyX U200 cement with no priming. However, after primer application, RelyX U200 showed higher bond strength compared to G-Cem linkace cement. After a thermocycling procedure, the bond strength values of specimens using G-Cem linkace cement were decreased significantly. On the other hand, the bond strength values of RelyX U200 specimens were increased. Primer application promoted high bond strength and less effect on bond strength reduction after thermocycling regardless of type of cement, zirconia block, or aging time. Most specimens showed adhesive failure and mixed failure, with adhesive failure occurring in the highest proportion. Only a small number of specimens showed mixed failure. In the Ce-TZP block, the PU group where RelyX U200 was used with primer application showed the highest percentage of mixed failure before thermocycling. No significant association was observed between the failure patterns and the shear bond strength (Figure 3).
4. Discussion This study evaluated the shear bond strength of resin cement to Y-TZP and Ce-TZP/Al2 O3 depending on whether a primer and/or thermocycling procedure is applied. The importance of air-abrasion in order to achieve a stable and high bond strength to zirconia surfaces has been shown in a previous study , and consequently that protocol was included in this study. Air-abrasion increases the surface area and wettability of oxide ceramics such as zirconia by making the surface rougher and consequently improves the bond strength to
resin cement. Air-abrasion also removes organic contaminants . Z-Prime Plus contains phosphate monomer and carboxylate monomer. The phosphate monomer bonds with metal oxides such as zirconia . Carboxylate groups in Z-Prime Plus reinforce the adhesion to zirconia. When a primer including phosphorylated monomer is applied to zirconia, the bond strength is improved, and the primer also acts as a wetting agent for the resin cement. The two resin cement types used in the current study are self-adhesive resin cement, which do not require the use of additional adhesives or primers, thereby saving time and effort. In general, self-adhesive resin cement is known to show weaker bond strength compared to self-etching resin cement or total etching resin cement . However, because it contain MDP, it reacts chemically with metal oxide and shows relatively high bond strength . This study showed that the shear bond strength of the NG groups is high, and group NU has low bond strength for 3day specimens. There seems to be a difference in filler content and viscosity between the two cement types. G-Cem linkace cement was not significantly influenced by the application of primer unlike RelyX U200. When G-Cem linkace cement was used for Y-TZP cementation, there was not any difference in bond strength depending on primer application. On the other hand, the bond strength of RelyX U200 cement significantly improved after primer application. When primer was applied, there was a significant difference in bond strength according to the different resin cement types. Because RelyX U200 resin cement has higher filler content and viscosity, primer application to zirconia increased its wettability and allowed easier penetration of the resin cement . Another study also reported that primer application dramatically increases the bond strength when RelyX U200 is used . This is consistent with previous studies [27, 32] and shows that both air-abrasion and primer application contribute to effective
BioMed Research International bonding. On the other hand, contradictory results on primer application can be found. A previous study reported that primer application did not have any effect on bond strength to air-abraded Y-TZP surfaces . In other studies, the bond strength significantly improved after air-abrasion with 50𝜇m Al2 O3 particles, and air-abrasion was a more significant factor than primer application [33, 34]. G-Cem linkace cement received more impact from thermocycling. Although whole groups using G-Cem linkace cement showed high shear bond strength in the 3-day groups, it was decreased after the thermocycling procedure. The primer treated group exhibited a slight decrease, and the nonpriming group showed a sharp decrease of bond strength. In contrast, there was a slightly different aspect in the groups using RelyX U200 cement. Group PU of the Y-TZP block demonstrated a significantly high elevation of bond strength after 5,000 times thermocycling. Although there was no significant difference, the Ce-TZP/Al2 O3 block showed a slight increase of bond strength. Group NU specimens did not exhibit a significant difference between the 3-day and 5,000 times thermocycling groups. As opposed to the groups using G-Cem linkace cement that showed reduced bond strength, it was a different pattern. This aspect has been reported in several previous papers. It is known that RelyX U200 has moisture tolerance and contributes by complete polymerization of the chemically cured part during thermocycling . In the comparison of the type of zirconia blocks, the YTZP block has higher bond strength compared with the CeTZP/Al2 O3 block. Through the SEM pictures, it was difficult to find significant differences between the two blocks on the surface of the specimens having undergone air-abrasion to 3.5 bar; it is considered that there are close associations with a difference in composition. In the case of Ce-TZP/Al2 O3 , not only does it consist of mere zirconia, but also it forms a nanocomposite with Al2 O3 for optimal fracture strength. So, there is some possibility that the differences of bond strength were influenced by the material composition. The possibility exists of an interaction between the Ce-TZP/Al2 O3 nanocomposite and the powder for air-abrasion including Al2 O3 as well. Ce-TZP/Al2 O3 is known to be more sensitive to stress-induced transformation , and the transformation after air-abrasion probably changed the surface and affected the bond strength. The necessity for more in-depth scientific research may be considered in the field of Ce-TZP/Al2 O3 materials itself. In this study, 3.5-bar pressure was used for air-abrasion using previous studies as [37–39]. Hallmann et al.  reported that as the pressure of air-abrasion increased, greater surface changes occurred and the surface became rougher. A rougher surface results in more microretentive area and allows for mechanical interlocking with the resin cement. In the SEM image, intergrain space is observed in the abraded zirconia surface . Air-abrasion treatment forms more hydroxyl groups on the ceramic surface and enhances the chemical reaction with MDP . Several studies have reported that air-abrasion with high pressure damages the zirconia surface and deteriorates its mechanical properties. In order to minimize surface damage,
5 air-abrasion with low pressure should be used, and a phosphate monomer containing primer is needed for a durable bond [41, 42]. Yang et al.  reported that air-abrasion with 2.5-bar pressure increases the surface roughness, increases the wettability of resin cement without additional primer application, and allows MDP within the resin cement to contribute to high bond strength. Conversely, if abrasion is performed with a low pressure of 0.5 bar and primer is not applied, significantly lower bond strength was achieved. If MDP-containing primer is used after the same low pressure air-abrasion treatment, significantly higher bond strength was obtained. The primer application compensated for the difference in surface roughness due to the different airabrasion pressure. According to these results, if low pressure air-abrasion is used or resin cement without functional groups is used, primer application is significant for achieving high bond strength. As reported by Hallmann et al. , airabrasion may increase the chance of surface cracks or surface damage despite increasing the roughness. Therefore, it may clinically worsen the prognosis of zirconia restoration For further evaluation, additional experiments with greater numbers of specimens are needed. Because adhesion studies on Ce-TZP/Al2 O3 are scarce, further studies to find the optimal adhesion protocol depending on the pressure used for air-abrasion and primer application are needed. In addition, the phase transformation of Ce-TZP/Al2 O3 after air-abrasion and the consequent change in fracture resistance and bond strength should be investigated.
5. Conclusions Depending on the type of the primer or resin cement used after air-abrasion, different wettability on zirconia surfaces can be observed. Application of primer affected the values of shear bond strength after a thermocycling procedure. In the case of using the same bonding protocol, the Y-TZP block could obtain higher bond strength compared with the CeTZP/Al2 O3 block.
Competing Interests The authors have no potential conflict of interests to declare.
Authors’ Contributions Jong-Eun Kim and Jee-Hwan Kim equally contributed to this work as first authors.
Acknowledgments This research was supported by a faculty research grant from Yonsei University College of Dentistry (6-2015-0104).
References  B. G¨okc¸en-R¨ohlig, A. Saruhanoglu, E. D. Cifter, and G. Evlioglu, “Applicability of zirconia dental prostheses for metal allergy patients,” The International Journal of Prosthodontics, vol. 23, no. 6, pp. 562–565, 2010.
6  P. Pittayachawan, A. McDonald, A. Petrie, and J. C. Knowles, “The biaxial flexural strength and fatigue property of Lava YTZP dental ceramic,” Dental Materials, vol. 23, no. 8, pp. 1018– 1029, 2007.  I. Denry and J. R. Kelly, “State of the art of zirconia for dental applications,” Dental Materials, vol. 24, no. 3, pp. 299–307, 2008.  P. Magne, M. P. G. Paranhos, and L. H. Burnett Jr., “New zirconia primer improves bond strength of resin-based cements,” Dental Materials, vol. 26, no. 4, pp. 345–352, 2010.  R. G. Luthardt, O. Sandkuhl, and B. Reitz, “Zirconia-TZP and alumina—advanced technologies for the manufacturing of single crowns,” The European Journal of Prosthodontics and Restorative Dentistry, vol. 7, no. 4, pp. 113–119, 1999.  M. Ferraris, E. Vern´e, P. Appendino et al., “Coatings on zirconia for medical applications,” Biomaterials, vol. 21, no. 8, pp. 765– 773, 2000.  J. Y. Thompson, B. R. Stoner, J. R. Piascik, and R. Smith, “Adhesion/cementation to zirconia and other non-silicate ceramics: where are we now?” Dental Materials, vol. 27, no. 1, pp. 71–82, 2011.  P. Kohorst, L. Borchers, J. Strempel et al., “Low-temperature degradation of different zirconia ceramics for dental applications,” Acta Biomaterialia, vol. 8, no. 3, pp. 1213–1220, 2012.  T. Kosmaˇc, C. Oblak, P. Jevnikar, N. Funduk, and L. Marion, “The effect of surface grinding and sandblasting on flexural strength and reliability of Y-TZP zirconia ceramic,” Dental Materials, vol. 15, no. 6, pp. 426–433, 1999.  C. Piconi and G. Maccauro, “Zirconia as a ceramic biomaterial,” Biomaterials, vol. 20, no. 1, pp. 1–25, 1999.  M. Nawa, S. Nakamoto, T. Sekino, and K. Niihara, “Tough and strong Ce-TZP/alumina nanocomposites doped with titania,” Ceramics International, vol. 24, no. 7, pp. 497–506, 1998.  K. Tanaka, J. Tamura, K. Kawanabe et al., “Ce-TZP/Al2 O3 nanocomposite as a bearing material in total joint replacement,” Journal of Biomedical Materials Research, vol. 63, no. 3, pp. 262– 270, 2002.  G. A. Borges, A. M. Sophr, M. F. de Goes, L. C. Sobrinho, and D. C. N. Chan, “Effect of etching and airborne particle abrasion on the microstructure of different dental ceramics,” Journal of Prosthetic Dentistry, vol. 89, no. 5, pp. 479–488, 2003.  A. Della Bona, M. Borba, P. Benetti, and D. Cecchetti, “Effect of surface treatments on the bond strength of a zirconia-reinforced ceramic to composite resin,” Brazilian Oral Research, vol. 21, no. 1, pp. 10–15, 2007. ¨  M. Ozcan, H. Nijhuis, and L. F. Valandro, “Effect of various surface conditioning methods on the adhesion of dual-cure resin cement with MDP functional monomer to zirconia after thermal aging,” Dental Materials Journal, vol. 27, no. 1, pp. 99– 104, 2008.  W. Awliya, A. Od´en, P. Yaman, J. B. Dennison, and M. E. Razzoog, “Shear bond strength of a resin cement to densely sintered high-purity alumina with various surface conditions,” Acta Odontologica Scandinavica, vol. 56, no. 1, pp. 9–13, 1998.  J.-H. Phark, S. Duarte Jr., M. Blatz, and A. Sadan, “An in vitro evaluation of the long-term resin bond to a new densely sintered high-purity zirconium-oxide ceramic surface,” Journal of Prosthetic Dentistry, vol. 101, no. 1, pp. 29–38, 2009.  M. B. Blatz, M. Bergler, F. Ozer, S. Holst, J.-H. O. Phark, and G. J. Chiche, “Bond strength of different veneering ceramics to zirconia and their susceptibility to thermocycling,” American Journal of Dentistry, vol. 23, no. 4, pp. 213–216, 2010.
BioMed Research International  M. B. Blatz, G. Chiche, S. Holst, and A. Sadan, “Influence of surface treatment and simulated aging on bond strengths of luting agents to zirconia,” Quintessence International, vol. 38, no. 9, pp. 745–753, 2007.  G. Yang, J.-C. Li, G.-C. Wang, M. Yashima, S.-L. Min, and T.-C. Chen, “Investigation on strengthening and toughening mechanisms of Ce-TZP/Al2 O3 nanocomposites,” Metallurgical and Materials Transactions A: Physical Metallurgy and Materials Science, vol. 37, no. 6, pp. 1969–1975, 2006.  S. Ban, H. Sato, Y. Suehiro, H. Nakanishi, and M. Nawa, “Biaxial flexure strength and low temperature degradation of Ce-TZP/Al2 O3 nanocomposite and Y-TZP as dental restoratives,” Journal of Biomedical Materials Research—Part B Applied Biomaterials, vol. 87, no. 2, pp. 492–498, 2008.  R. V. Mangalaraja, B. K. Chandrasekhar, and P. Manohar, “Effect of ceria on the physical, mechanical and thermal properties of yttria stabilized zirconia toughened alumina,” Materials Science and Engineering A, vol. 343, no. 1-2, pp. 71–75, 2003.  J. Fischer and B. Stawarczyk, “Compatibility of machined CeTZP/Al2 O3 nanocomposite and a veneering ceramic,” Dental Materials, vol. 23, no. 12, pp. 1500–1505, 2007.  M. Hirano and H. Inada, “Fracture toughness, strength and Vickers hardness of yttria-ceria-doped tetragonal zirconia/alumina composites fabricated by hot isostatic pressing,” Journal of Materials Science, vol. 27, no. 13, pp. 3511–3518, 1992.  R. Benzaid, J. Chevalier, M. Saˆadaoui et al., “Fracture toughness, strength and slow crack growth in a ceria stabilized zirconiaalumina nanocomposite for medical applications,” Biomaterials, vol. 29, no. 27, pp. 3636–3641, 2008.  A. J. Raigrodski, “Contemporary materials and technologies for all-ceramic fixed partial dentures: a review of the literature,” Journal of Prosthetic Dentistry, vol. 92, no. 6, pp. 557–562, 2004.  M. Kern, “Resin bonding to oxide ceramics for dental restorations,” Journal of Adhesion Science and Technology, vol. 23, no. 7-8, pp. 1097–1111, 2009.  T. Derand, M. Molin, and K. Kvam, “Bond strength of composite luting cement to zirconia ceramic surfaces,” Dental Materials, vol. 21, no. 12, pp. 1158–1162, 2005.  B. Yang, A. Barloi, and M. Kern, “Influence of air-abrasion on zirconia ceramic bonding using an adhesive composite resin,” Dental Materials, vol. 26, no. 1, pp. 44–50, 2010.  J. Perdig˜ao, S. D. Fernandes, A. M. Pinto, and F. A. Oliveira, “Effect of artificial aging and surface treatment on bond strengths to dental zirconia,” Operative Dentistry, vol. 38, no. 2, pp. 168–176, 2013.  S.-H. Youm, K.-H. Jung, S.-A. Son, Y.-H. Kwon, and J.-K. Park, “Effect of dentin pretreatment and curing mode on the microtensile bond strength of self-adhesive resin cements,” Journal of Advanced Prosthodontics, vol. 7, no. 4, pp. 317–322, 2015.  Y.-J. Shin, Y. Shin, Y.-A. Yi et al., “Evaluation of the shear bond strength of resin cement to Y-TZP ceramic after different surface treatments,” Scanning, vol. 36, no. 5, pp. 479–486, 2014.  L. Miragaya, L. C. Maia, C. E. Sabrosa, M. F. de Goes, and E. M. da Silva, “Evaluation of self-adhesive resin cement bond strength to yttria-stabilized zirconia ceramic (Y-TZP) using four surface treatments,” The Journal of Adhesive Dentistry, vol. 13, no. 5, pp. 473–480, 2011.  Y. A. Yi, J. S. Ahn, Y. J. Park et al., “The effect of sandblasting and different primers on shear bond strength between yttriatetragonal zirconia polycrystal ceramic and a self-adhesive resin cement,” Operative Dentistry, vol. 40, no. 1, pp. 63–71, 2015.
BioMed Research International  K. Bitter, H. Meyer-Lueckel, K. Priehn, J. P. Kanjuparambil, K. Neumann, and A. M. Kielbassa, “Effects of luting agent and thermocycling on bond strengths to root canal dentine,” International Endodontic Journal, vol. 39, no. 10, pp. 809–818, 2006.  H. Sato, K. Yamada, G. Pezzotti, M. Nawa, and S. Ban, “Mechanical properties of dental zirconia ceramics changed with sandblasting and heat treatment,” Dental Materials Journal, vol. 27, no. 3, pp. 408–414, 2008.  J.-S. Ahn, Y.-A. Yi, Y. Lee, and D.-G. Seo, “Shear bond strength of MDP-containing self-adhesive resin cement and Y-TZP ceramics: effect of phosphate monomer-containing primers,” BioMed Research International, vol. 2015, Article ID 389234, 6 pages, 2015.  D. Liu, J. P. Matinlinna, J. K.-H. Tsoi et al., “A new modified laser pretreatment for porcelain zirconia bonding,” Dental Materials, vol. 29, no. 5, pp. 559–565, 2013.  H. R. Sarmento, F. Campos, R. S. Sousa et al., “Influence of air-particle deposition protocols on the surface topography and adhesion of resin cement to zirconia,” Acta Odontologica Scandinavica, vol. 72, no. 5, pp. 346–353, 2014.  L. Hallmann, P. Ulmer, E. Reusser, and C. H. F. H¨ammerle, “Effect of blasting pressure, abrasive particle size and grade on phase transformation and morphological change of dental zirconia surface,” Surface and Coatings Technology, vol. 206, no. 19-20, pp. 4293–4302, 2012.  A. Attia and M. Kern, “Effect of cleaning methods after reducedpressure air abrasion on bonding to zirconia ceramic,” The Journal of Adhesive Dentistry, vol. 13, no. 6, pp. 561–567, 2011.  A. Attia, F. Lehmann, and M. Kern, “Influence of surface conditioning and cleaning methods on resin bonding to zirconia ceramic,” Dental Materials, vol. 27, no. 3, pp. 207–213, 2011.